# Chapter 7. Highlights:

Save this PDF as:

Size: px
Start display at page:

## Transcription

1 Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true strain, strain exponent, and know the difference between elastic and plastic deformation.. Understand what a stress-strain curve is and what information it contains about materials properties. Be able to identify and/or calculate all the properties in #1 from a stress-strain curve, both in the elastic and plastic (before necking) regions. 3. Understand how the mechanical behavior of ceramics differs from that of metals. Be able to numerically manipulate the flexural strength and the effect of porosity on mechanical strength. 4. Understand how the mechanical behavior of polymers differs from that of metals. Understand and be able to numerically manipulate the viscoelastic modulus. Notes: Show Figures 7.1 to 7.4.

2 Define engineering stress and strain (tension and compression): Engineering stress F A Engineering strain ε l i - l l l l

3 For shear stress, Shear stress τ F A Shear strain γ tanθ ( θ is strain angle) As shown in Figure 7.4, and described in Equations 7.4a and 7.4b, an applied axial force can be geometrically decomposed into tensile and shear components. Stress-strain test: slowly increase stress and measure strain until the material fractures (show Figures 7., 7.3, 7.5, 7.1-1). These tests are usually performed in tension. In the linear portion of the curve, Hooke's law is obeyed, Eε. E is called the modulus of elasticity, or Young's modulus, and is a property of the material. The units of E are psi or MPa, remembering that PaN/m. Typical values for E are given in Table 7.1 for metals, ceramics and polymers.

4

5

6 A similar relationship can be written for compressive, shear, and torsional loads. For shear stress, τ G γ G is the shear modulus and is a property of the material. On an atomic scale, lengthening (compressing) a specimen during tensile (compressive) loading results in lengthening (shortening) of atomic bonds. Young's modulus is a measure of the resistance to separation of adjacent atoms. Youngs modulus df dr r Show Figure 7.7 and Table 7.1. High E- W and Ni, low E- Mg, Al, Au, Ag. Show Table 3.7. E can be different in different directions, and this reflects the different atomic densities in different planes and directions. When there is not a significant linear portion of an engineering stressstrain diagram, the secant and tangent modulus are sometimes employed. Show Figure 7.6. The tangent modulus is the slope of the stressstrain curve at one particular point, while the secant modulus is the slope of a secant drawn from the origin to a particular point on the stressstrain curve. By common sense, tensile strain in the z direction should yield compressive strain in the x and y directions. Show Figure 7.9. ε x ε y. Define Poisson's ratio υ ε ε y ν - x - ε z ε z υ for most metals, and is again a property of the material. It can be shown that G.4E for most metals. E G(1+ ν ) The following analogies illustrate the differences between the linear and nonlinear portions of a stress-strain curve:

7 Hooke's law Bonds stretched Elastic deformation No permanent damage Nonlinear -ε Bonds broken Plastic deformation Permanent damage Example Problem A cylindrical steel bar 1 mm in diameter is to be elastically deformed. Using the data in Table 7.1, determine the force needed to produce a reduction of 3x1-3 mm in the diameter. From Table 7.1, E 7 GPa and ν.3. We are given information about the desired radial strain: ε r 3 3x1 mm 4 3x1 1 mm This can be related to the axial strain by the definition of Poisson s ratio, eq. 7.8: ε z 4 3x1 3 ε r 1x1 υ.3 Now use Hooke s law, eq. 7.5, to determine the stress that must be applied: 3 ( 1x1 ).7GPa MPa Eε (7GPa) 7 From the definition of stress, eq. 7.3, F 6 π A 7 x1 Pa (.1m) 1.63x1 4 4 N Tensile Properties of Materials: Show a stress-strain curve, Figure 7.1. We will now digress for a while but eventually return to this figure and try to understand it and extract useful information. The linear portion of this curve undergoes elastic deformation (linear -ε), which disappears after the stress is removed. In other words, it is reversible. When the stress exceeds the linear portion of the stress-strain curve, permanent (irreversible) plastic deformation occurs. Plastic deformation Plastic deformation usually occurs near ε.5 for metals. When Hooke's law fails, the material undergoes plastic deformation. Show Figure 7.1. Either 7.1a or 7.1b can occur, usually 7.1a. Since plastic deformation involves atomic-level breaking of bonds and reforming of new ones, it is irreversible. We want to be able to define unambiguously when a material yields, when it is permanently damaged. Show Figure 7.1a, focusing on point P. This is the proportional limit, where the stress-strain curve deviates from linearity. But this is ambiguous.

8 Usually the stress-strain curve deviates from linearity quite gradually, so we need to define an arbitrary but universal definition of the elastic region. Starting from point, ε., draw a parallel line to the linear portion of the stress-strain curve. The stress at which this line intersects with the stress-strain curve is called the yield strength, y. This is one measure of a material's strength, its ability to resist plastic (permanent) deformation. In the case of Figure 7.1b the yield strength is the lower yield point. Show Figure The tensile strength is defined as the maximum stress prior to fracture. After M, "necking" occurs, the cross-sectional area shrinks abruptly. The ductility is defined as the % plastic deformation at fracture. Ductility A low ductility material is brittle. Show Figure l f - l l x1 Resilience is the capability of a material to absorb energy when it is deformed elastically. The modulus of resilience U r is ε y U r dε where ε y is the strain at fracture. Show Figure For linear stress-strain curve, U r 1 y ε y y E Toughness is the ability of a material to absorb energy up to fracture. It is defined by the same integral as U r above, but the upper limit of integration is now fracture instead of yielding. Show Table 7.3. High ductility corresponds somewhat with low strength. Example Problem For a given set of data, which I will not reproduce here, you should be able to: a) Create a plot of engineering stress versus engineering strain, b) determine the elastic modulus, c) determine the yield strength, d) determine the tensile strength, e) determine the ductility, and f) determine the modulus of resilience. a) The plots below were obtained by taking: F( N ) F( N ) ( Pa ) π π 3 D ( 1.8x1 m) F( N )

9 ε l i i l l l e8 Stress (Pa).e8 1.e8.e Strain b) The elastic modulus is taken as the slope of the linear portion of the curve. Looking at the nd plot, which focuses on the linear portion of the curve, take the average slope only from the 1 st four points. This yields: x1 Pa 1.173x1 Pa 1.795x1 Pa E ε x1 Pa.398 Taking the average of these 4 values yields E 5.88x1 1 Pa. c) On the nd plot, draw a line from ε. with a slope of E 5.88x1 1 Pa. The intersection of this line with the -ε curve gives y.8x1 8 Pa. d) From the 1 st plot, the maximum in is the tensile strength 3.7x1 8 Pa. e) From the 1 st plot, the strain at failure is about.145, subtract out the elastic strain (.5) to get the plastic strain of.14. Thus the ductility is 14%.

10 f) Determine the modulus of resilience from equation 7.14: U r y E Elastic recovery after plastic deformation: Show figure 7.17 and discuss. 8 (.8x1 Pa) (5.88x1 1 Pa) 6.67x1 5 Pa True Stress and Strain: True stress( T ) and true strain(ε T ) are defined similarly to engineering stress and strain. T F A i Force Instantaneous area ε l ln l T i l i is the instantaneous length If volume is conserved, then A i l i A l and T (1 + ε ) ε T ln (1 + ε ) The above two equations are only true until necking. After necking, true stress and true strain can only be

11 determined by actual measurements. Show Figure 7.16, where the true stress is corrected to account for nontensile components. For some metals, from the onset of plastic deformation to the point at which necking begins, the true stress is approximately: n T K ε T K and n, the strain hardening exponent, vary across different metals and alloys. Example Problem You are given that just prior to necking, (, ε) (35 MPa,.194) and (5 MPa,.96). What value of will produce ε.5. In order to use equation (7.19), we need to convert from engineering stress and strain to true stress and strain. From equations (7.18) 1 T (1+ ε ) MPa T (1+ ε ) 34 MPa 1 ε T ln(1+ ε ).1773 ε T ln(1+ ε ) ε T ln(1+ ε ).31 You need to use equation (7.19) to setup two equations with two unknowns. Taking the ln of both sides: ln(34 ln ln K + nlnε T MPa ) ln K + n ln(.593) T

12 ln(8.59 MPa ) ln K + n ln(.1773) Subtracting the nd from the 1 st ln n ln Substituting back into above: n.378 ln (8.59 MPa ) ln K + (.378) ln(.1773) ln K 6.91 or K 54 MPa Now find where ε T is.31: n T K ε T.378 T (54 MPa)(.31) MPa Convert back to engineering stress: T 1 + ε 36.3 MPa MPa Mechanical behavior: Ceramics Ceramic materials are less mechanically useful than metals because they are generally quite brittle. Their mechanical strength is not normally assessed by tensile stress-strain measurements. It is extremely difficult to prepare the proper sample geometry, the samples generally crack when gripped, and their strain at failure is too small to accurately measure. Show Figure For these reasons, the strength of ceramic materials is normally assessed by a traverse bending test. Show Figure The failure point is described by the flexural strength ( fs ), also known as the modulus of rupture( mr ). For rectangular cross sections, and for circular cross-sections: fs 3 F f L b d F f L π R fs 3

13

14 Example Problem A 3-point bending test is performed on Al O 3 with a circular cross-section of radius 3.5 mm. The specimen fractures at a load of 95 N when the support points are 5 mm apart. Consider a square sample of the same material with a square cross-section of 1mm on each edge. If the support points are 4 mm apart, at what load will the sample fracture? First, determine the flexural strength of this material from equation (7.b): fs F L 3 f (95 N )(5x1 m) 3.53x πr π (3.5x1 m) 8 Pa Now determine the failure force from equation (7.a): F bd 3 3 fs (1x1 m) 3 3L 3(4x1 (3.53x1 m) 8 Pa) 1,17 N Ceramic solids are often fabricated by compaction or foaming of ceramic particles. In this case, the ceramic solid may have considerable porosity, which degrades its strength. The modulus of elasticity (E) and the flexural strength ( fs ) depend on the volume fraction porosity (P) according to: ( 1 1.9P. P ) E E + 9 fs exp( np) where and n are experimental constants. Example Problem Using the data in Table 7., a) Determine the flexural strength of nonporous MgO assuming n 3.75 b) Calculate the volume fraction porosity when fs 6 MPa. a) Taking the ln of both sides of equation 7.: ln fs ln np From Table 7., fs 15MPa with 5% porosity, so ln(15 MPa ) ln (3.75)(.5) ln MPa

15 b) Rearranging the above equation: P ln ln fs n ln(6 MPa) P or 19vol.% Note that 5% porosity reduces fs by 17%, and 19% porosity reduces fs by 51%.

16 Mechanical behavior: Polymers Typical stress-strain diagrams for polymers are shown in Figure 7.. The behavior ranges from strong and brittle (curve A) to rubbery (curve C). The mechanical behavior of polymers is far more temperaturedependent than that of metals and polymers. Show Figure 7.4. Polymethyl methylacrylate behaves like a brittle metal at low temperature, but like an elastomer (rubber band) at low temperature. At intermediate temperatures, this polymer behaves like a viscoelastic material, which combines the behavior of a viscous and an elastic material. The most famous viscoelastic material is silly putty, which is intermediate between a liquid and a solid. Show Figure 7.6, which shows the strain behavior with time following instantaneous application of a load. Alternatively, one can study the mechanical behavior of a viscoelastic material at constant strain, in which case the stress that is initially applied will gradually decrease. Show Figure 7.7, which shows the stress as a function of time and temperature. How can we compare different materials?? One way is to choose an arbitrary time (1 sec is common) and define the relaxation modulus, E r (t), at that time: E r ( t) ( t) ε Remember that the value of E r (1) depends on the temperature. Show Figure 7.7 again.

17 Safety factor Engineering with a safety factor accounts for material variability, nonideal conditions, human error, etc. and is common engineering practice. The working stress ( w ) is reduced from the yield stress ( y ) by the safety factor (N) according to: The safety factor N is commonly taken as. y w N

### Introduction to Engineering Materials ENGR2000. Dr. Coates

Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed

### ME 2570 MECHANICS OF MATERIALS

ME 2570 MECHANICS OF MATERIALS Chapter III. Mechanical Properties of Materials 1 Tension and Compression Test The strength of a material depends on its ability to sustain a load without undue deformation

### Outline. Tensile-Test Specimen and Machine. Stress-Strain Curve. Review of Mechanical Properties. Mechanical Behaviour

Tensile-Test Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress - true strain (flow curve) mechanical properties: - Resilience - Ductility - Toughness - Hardness A standard

### Stress-Strain Behavior

Stress-Strain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.

### ME 243. Mechanics of Solids

ME 243 Mechanics of Solids Lecture 2: Stress and Strain Ahmad Shahedi Shakil Lecturer, Dept. of Mechanical Engg, BUET E-mail: sshakil@me.buet.ac.bd, shakil6791@gmail.com Website: teacher.buet.ac.bd/sshakil

### Mechanical Properties of Materials

Mechanical Properties of Materials Strains Material Model Stresses Learning objectives Understand the qualitative and quantitative description of mechanical properties of materials. Learn the logic of

### Tensile stress strain curves for different materials. Shows in figure below

Tensile stress strain curves for different materials. Shows in figure below Furthermore, the modulus of elasticity of several materials effected by increasing temperature, as is shown in Figure Asst. Lecturer

### NORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.

NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric

### Module-4. Mechanical Properties of Metals

Module-4 Mechanical Properties of Metals Contents ) Elastic deformation and Plastic deformation ) Interpretation of tensile stress-strain curves 3) Yielding under multi-axial stress, Yield criteria, Macroscopic

### CHAPTER 7 MECHANICAL PROPERTIES PROBLEM SOLUTIONS

Excerpts from this work may be reproduced by instructors for distribution on a not-for-profit basis for testing or instructional purposes only to students enrolled in courses for which the textbook has

### Chapter 6: Mechanical Properties of Metals. Dr. Feras Fraige

Chapter 6: Mechanical Properties of Metals Dr. Feras Fraige Stress and Strain Tension Compression Shear Torsion Elastic deformation Plastic Deformation Yield Strength Tensile Strength Ductility Toughness

### STANDARD SAMPLE. Reduced section " Diameter. Diameter. 2" Gauge length. Radius

MATERIAL PROPERTIES TENSILE MEASUREMENT F l l 0 A 0 F STANDARD SAMPLE Reduced section 2 " 1 4 0.505" Diameter 3 4 " Diameter 2" Gauge length 3 8 " Radius TYPICAL APPARATUS Load cell Extensometer Specimen

### 6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and

6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile

### CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS

CHAPTER 6 MECHANICAL PROPERTIES OF METALS PROBLEM SOLUTIONS Concepts of Stress and Strain 6.1 Using mechanics of materials principles (i.e., equations of mechanical equilibrium applied to a free-body diagram),

### The science of elasticity

The science of elasticity In 1676 Hooke realized that 1.Every kind of solid changes shape when a mechanical force acts on it. 2.It is this change of shape which enables the solid to supply the reaction

### MECE 3321 MECHANICS OF SOLIDS CHAPTER 3

MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.

### Mechanical properties 1 Elastic behaviour of materials

MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical

### , to obtain a way to calculate stress from the energy function U(r).

BIOEN 36 014 LECTURE : MOLECULAR BASIS OF ELASTICITY Estimating Young s Modulus from Bond Energies and Structures First we consider solids, which include mostly nonbiological materials, such as metals,

### INTRODUCTION TO STRAIN

SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,

### 4.MECHANICAL PROPERTIES OF MATERIALS

4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stress-strain diagram

### EMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain - Axial Loading

MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain - Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain - Axial Loading Statics

### ME 207 Material Science I

ME 207 Material Science I Chapter 3 Properties in Tension and Compression Dr. İbrahim H. Yılmaz http://web.adanabtu.edu.tr/iyilmaz Automotive Engineering Adana Science and Technology University Introduction

### [5] Stress and Strain

[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law

### MATERIALS FOR CIVIL AND CONSTRUCTION ENGINEERS

MATERIALS FOR CIVIL AND CONSTRUCTION ENGINEERS 3 rd Edition Michael S. Mamlouk Arizona State University John P. Zaniewski West Virginia University Solution Manual FOREWORD This solution manual includes

### 12/8/2009. Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka

Prof. A.K.M.B. Rashid Department of MME BUET, Dhaka Introduction and classes of properties Case studies showing selection of the right material for the job Deformation of material under the action of a

### Solid Mechanics Chapter 1: Tension, Compression and Shear

Solid Mechanics Chapter 1: Tension, Compression and Shear Dr. Imran Latif Department of Civil and Environmental Engineering College of Engineering University of Nizwa (UoN) 1 Why do we study Mechanics

### Mechanical Properties of Polymers. Scope. MSE 383, Unit 3-1. Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept.

Mechanical Properties of Polymers Scope MSE 383, Unit 3-1 Joshua U. Otaigbe Iowa State University Materials Science & Engineering Dept. Structure - mechanical properties relations Time-dependent mechanical

### The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties.

Objective: The objective of this experiment is to investigate the behavior of steel specimen under a tensile test and to determine it's properties. Introduction: Mechanical testing plays an important role

### UNIT I SIMPLE STRESSES AND STRAINS

Subject with Code : SM-1(15A01303) Year & Sem: II-B.Tech & I-Sem SIDDHARTH GROUP OF INSTITUTIONS :: PUTTUR Siddharth Nagar, Narayanavanam Road 517583 QUESTION BANK (DESCRIPTIVE) UNIT I SIMPLE STRESSES

### N = N A Pb A Pb. = ln N Q v kt. = kt ln v N

5. Calculate the energy for vacancy formation in silver, given that the equilibrium number of vacancies at 800 C (1073 K) is 3.6 10 3 m 3. The atomic weight and density (at 800 C) for silver are, respectively,

### Samantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2

Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force

### CHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS

CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a cross-sectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress

### STRENGTH OF MATERIALS-I. Unit-1. Simple stresses and strains

STRENGTH OF MATERIALS-I Unit-1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between

### MECHANICS OF MATERIALS

Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:

### How materials work. Compression Tension Bending Torsion

Materials How materials work Compression Tension Bending Torsion Elemental material atoms: A. Composition a) Nucleus: protons (+), neutrons (0) b) Electrons (-) B. Neutral charge, i.e., # electrons = #

### Advanced Structural Analysis EGF Section Properties and Bending

Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear

### High Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?

High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the

### Module 5: Failure Criteria of Rock and Rock masses. Contents Hydrostatic compression Deviatoric compression

FAILURE CRITERIA OF ROCK AND ROCK MASSES Contents 5.1 Failure in rocks 5.1.1 Hydrostatic compression 5.1.2 Deviatoric compression 5.1.3 Effect of confining pressure 5.2 Failure modes in rocks 5.3 Complete

### MATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?

MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition

### Laboratory 4 Bending Test of Materials

Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective

### Johns Hopkins University What is Engineering? M. Karweit MATERIALS

Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: MATERIALS A. Composition

### 9 MECHANICAL PROPERTIES OF SOLIDS

9 MECHANICAL PROPERTIES OF SOLIDS Deforming force Deforming force is the force which changes the shape or size of a body. Restoring force Restoring force is the internal force developed inside the body

### INTRODUCTION (Cont..)

INTRODUCTION Name : Mohamad Redhwan Abd Aziz Post : Lecturer @ DEAN CENTER OF HND STUDIES Subject : Solid Mechanics Code : BME 2033 Room : CENTER OF HND STUDIES OFFICE H/P No. : 019-2579663 W/SITE : Http://tatiuc.edu.my/redhwan

### Structural Analysis I Chapter 4 - Torsion TORSION

ORSION orsional stress results from the action of torsional or twisting moments acting about the longitudinal axis of a shaft. he effect of the application of a torsional moment, combined with appropriate

### 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?

IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at

### Theory at a Glance (for IES, GATE, PSU)

1. Stress and Strain Theory at a Glance (for IES, GATE, PSU) 1.1 Stress () When a material is subjected to an external force, a resisting force is set up within the component. The internal resistance force

### Module 5: Theories of Failure

Module 5: Theories of Failure Objectives: The objectives/outcomes of this lecture on Theories of Failure is to enable students for 1. Recognize loading on Structural Members/Machine elements and allowable

### ELASTICITY (MDM 10203)

ELASTICITY () Lecture Module 3: Fundamental Stress and Strain University Tun Hussein Onn Malaysia Normal Stress inconstant stress distribution σ= dp da P = da A dimensional Area of σ and A σ A 3 dimensional

### Elastic Properties of Solid Materials. Notes based on those by James Irvine at

Elastic Properties of Solid Materials Notes based on those by James Irvine at www.antonine-education.co.uk Key Words Density, Elastic, Plastic, Stress, Strain, Young modulus We study how materials behave

### Geology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)

Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties: - elastic modulii Outline of this Lecture 1. Uniaxial rock

### Mechanics of Materials Primer

Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus

### Agricultural Science 1B Principles & Processes in Agriculture. Mike Wheatland

Agricultural Science 1B Principles & Processes in Agriculture Mike Wheatland (m.wheatland@physics.usyd.edu.au) Outline - Lectures weeks 9-12 Chapter 6: Balance in nature - description of energy balance

### 13 Solid materials Exam practice questions

Pages 206-209 Exam practice questions 1 a) The toughest material has the largest area beneath the curve the answer is C. b) The strongest material has the greatest breaking stress the answer is B. c) A

### Lab Exercise #5: Tension and Bending with Strain Gages

Lab Exercise #5: Tension and Bending with Strain Gages Pre-lab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material

### N = Shear stress / Shear strain

UNIT - I 1. What is meant by factor of safety? [A/M-15] It is the ratio between ultimate stress to the working stress. Factor of safety = Ultimate stress Permissible stress 2. Define Resilience. [A/M-15]

### Stress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus. Case study

Stress Strain Elasticity Modulus Young s Modulus Shear Modulus Bulk Modulus Case study 2 In field of Physics, it explains how an object deforms under an applied force Real rigid bodies are elastic we can

### Constitutive Equations (Linear Elasticity)

Constitutive quations (Linear lasticity) quations that characterize the physical properties of the material of a system are called constitutive equations. It is possible to find the applied stresses knowing

### Lab Exercise #3: Torsion

Lab Exercise #3: Pre-lab assignment: Yes No Goals: 1. To evaluate the equations of angular displacement, shear stress, and shear strain for a shaft undergoing torsional stress. Principles: testing of round

### COMPLEX STRESS TUTORIAL 4 THEORIES OF FAILURE. You should judge your progress by completing the self assessment exercises.

COMPLEX STRESS TUTORIAL 4 THEORIES OF FAILURE This short tutorial covers no known elements of the E.C. or Edexcel Exams but should be studied as part of complex stress, structures and materials. You should

### Mechanics of Earthquakes and Faulting

Mechanics of Earthquakes and Faulting Lectures & 3, 9/31 Aug 017 www.geosc.psu.edu/courses/geosc508 Discussion of Handin, JGR, 1969 and Chapter 1 Scholz, 00. Stress analysis and Mohr Circles Coulomb Failure

### Materials and Structures. Indian Institute of Technology Kanpur

Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional

### Chapter Two: Mechanical Properties of materials

Chapter Two: Mechanical Properties of materials Time : 16 Hours An important consideration in the choice of a material is the way it behave when subjected to force. The mechanical properties of a material

### Mechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering

Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected

### Structural Metals Lab 1.2. Torsion Testing of Structural Metals. Standards ASTM E143: Shear Modulus at Room Temperature

Torsion Testing of Structural Metals Standards ASTM E143: Shear Modulus at Room Temperature Purpose To determine the shear modulus of structural metals Equipment Tinius-Olsen Lo-Torq Torsion Machine (figure

### COURSE TITLE : THEORY OF STRUCTURES -I COURSE CODE : 3013 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6

COURSE TITLE : THEORY OF STRUCTURES -I COURSE CODE : 0 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6 TIME SCHEDULE Module Topics Period Moment of forces Support reactions Centre

### Lecture #2: Split Hopkinson Bar Systems

Lecture #2: Split Hopkinson Bar Systems by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering, Chair of Computational Modeling of Materials in Manufacturing 2015 1 1 1 Uniaxial Compression

### Chapter 26 Elastic Properties of Materials

Chapter 26 Elastic Properties of Materials 26.1 Introduction... 1 26.2 Stress and Strain in Tension and Compression... 2 26.3 Shear Stress and Strain... 4 Example 26.1: Stretched wire... 5 26.4 Elastic

Fundamentals of Durability Page 1 Your single provider of solutions System simulation solutions 3D simulation solutions Test-based engineering solutions Engineering services - Deployment services Troubleshooting

### five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

### five Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture

ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS

### Strength of Materials (15CV 32)

Strength of Materials (15CV 32) Module 1 : Simple Stresses and Strains Dr. H. Ananthan, Professor, VVIET,MYSURU 8/21/2017 Introduction, Definition and concept and of stress and strain. Hooke s law, Stress-Strain

### Plasticity R. Chandramouli Associate Dean-Research SASTRA University, Thanjavur

Plasticity R. Chandramouli Associate Dean-Research SASTRA University, Thanjavur-613 401 Joint Initiative of IITs and IISc Funded by MHRD Page 1 of 9 Table of Contents 1. Plasticity:... 3 1.1 Plastic Deformation,

### 20. Rheology & Linear Elasticity

I Main Topics A Rheology: Macroscopic deformation behavior B Linear elasticity for homogeneous isotropic materials 10/29/18 GG303 1 Viscous (fluid) Behavior http://manoa.hawaii.edu/graduate/content/slide-lava

### ANSYS Mechanical Basic Structural Nonlinearities

Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria

### A concrete cylinder having a a diameter of of in. mm and elasticity. Stress and Strain: Stress and Strain: 0.

2011 earson Education, Inc., Upper Saddle River, NJ. ll rights reserved. This material is protected under all copyright laws as they currently 8 1. 3 1. concrete cylinder having a a diameter of of 6.00

### Sub. Code:

Important Instructions to examiners: ) The answers should be examined by key words and not as word-to-word as given in the model answer scheme. ) The model answer and the answer written by candidate may

### TENSILE TESTS (ASTM D 638, ISO

MODULE 4 The mechanical properties, among all the properties of plastic materials, are often the most important properties because virtually all service conditions and the majority of end-use applications

### Hardened Concrete. Lecture No. 16

Hardened Concrete Lecture No. 16 Fatigue strength of concrete Modulus of elasticity, Creep Shrinkage of concrete Stress-Strain Plot of Concrete At stress below 30% of ultimate strength, the transition

### Experiment Two (2) Torsional testing of Circular Shafts

Experiment Two (2) Torsional testing of Circular Shafts Introduction: Torsion occurs when any shaft is subjected to a torque. This is true whether the shaft is rotating (such as drive shafts on engines,

### Lecture 7, Foams, 3.054

Lecture 7, Foams, 3.054 Open-cell foams Stress-Strain curve: deformation and failure mechanisms Compression - 3 regimes - linear elastic - bending - stress plateau - cell collapse by buckling yielding

### Statics Principles. The laws of motion describe the interaction of forces acting on a body. Newton s First Law of Motion (law of inertia):

Unit 2 Review Statics Statics Principles The laws of motion describe the interaction of forces acting on a body Newton s First Law of Motion (law of inertia): An object in a state of rest or uniform motion

### In Situ Ultrasonic NDT of Fracture and Fatigue in Composites

ECNDT 26 - Mo.2.6.5 In Situ Ultrasonic NDT of Fracture and Fatigue in Composites I. SOLODOV, K. PFLEIDERER, and G. BUSSE Institute for Polymer Testing and Polymer Science (IKP), Non-destructive Testing

### EDEXCEL NATIONAL CERTIFICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQF LEVEL 3 OUTCOME 1 - LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS

EDEXCEL NATIONAL CERTIICATE/DIPLOMA MECHANICAL PRINCIPLES AND APPLICATIONS NQ LEVEL 3 OUTCOME 1 - LOADING SYSTEMS TUTORIAL 3 LOADED COMPONENTS 1. Be able to determine the effects of loading in static engineering

### Mechanics of Materials II. Chapter III. A review of the fundamental formulation of stress, strain, and deflection

Mechanics of Materials II Chapter III A review of the fundamental formulation of stress, strain, and deflection Outline Introduction Assumtions and limitations Axial loading Torsion of circular shafts

### 6.37 Determine the modulus of resilience for each of the following alloys:

6.37 Determine the modulus of resilience for each of the following alloys: Yield Strength Material MPa psi Steel alloy 550 80,000 Brass alloy 350 50,750 Aluminum alloy 50 36,50 Titanium alloy 800 116,000

### ME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam cross-sec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.

ME 323 - Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM-12:20PM Ghosh 2:30-3:20PM Gonzalez 12:30-1:20PM Zhao 4:30-5:20PM M (x) y 20 kip ft 0.2

### Design of a fastener based on negative Poisson's ratio foam adapted from

1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205-212 (1991).

### Mechanics of Earthquakes and Faulting

Mechanics of Earthquakes and Faulting www.geosc.psu.edu/courses/geosc508 Surface and body forces Tensors, Mohr circles. Theoretical strength of materials Defects Stress concentrations Griffith failure

### There are three main types of structure - mass, framed and shells.

STRUCTURES There are three main types of structure - mass, framed and shells. Mass structures perform due to their own weight. An example would be a dam. Frame structures resist loads due to the arrangement

### Lecture 4 Honeycombs Notes, 3.054

Honeycombs-In-plane behavior Lecture 4 Honeycombs Notes, 3.054 Prismatic cells Polymer, metal, ceramic honeycombs widely available Used for sandwich structure cores, energy absorption, carriers for catalysts

### MMJ1133 FATIGUE AND FRACTURE MECHANICS A - INTRODUCTION INTRODUCTION

A - INTRODUCTION INTRODUCTION M.N.Tamin, CSMLab, UTM Course Content: A - INTRODUCTION Mechanical failure modes; Review of load and stress analysis equilibrium equations, complex stresses, stress transformation,

### X has a higher value of the Young modulus. Y has a lower maximum tensile stress than X

Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which

### QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS

QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1- STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,

### CIVIL DEPARTMENT MECHANICS OF STRUCTURES- ASSIGNMENT NO 1. Brach: CE YEAR:

MECHANICS OF STRUCTURES- ASSIGNMENT NO 1 SEMESTER: V 1) Find the least moment of Inertia about the centroidal axes X-X and Y-Y of an unequal angle section 125 mm 75 mm 10 mm as shown in figure 2) Determine

### MECHANICS OF MATERIALS

GE SI CHAPTER 3 MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf David F. Mazurek Torsion Lecture Notes: J. Walt Oler Texas Tech University Torsional Loads on Circular Shafts

### QUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1- STRESS AND STRAIN PART A

DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1- STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State

### MAE 322 Machine Design. Dr. Hodge Jenkins Mercer University

MAE 322 Machine Design Dr. Hodge Jenkins Mercer University What is this Machine Design course really about? What you will learn: How to design machine elements 1) Design so they won t break under varying